1 DOI: 10.1002/admi.201700123
Article type: Full Paper
"This is the peer reviewed version of the following article: Mattinen et al., Adv. Mater. Interfaces, 4, 2017, 1700123, which has been published in final form at
https://doi.org/10.1002/admi.201700123. This article may be used for non-commercial purposes in accordance with Wiley Terms and Conditions for Use of Self-Archived Versions."
Atomic Layer Deposition of Crystalline MoS2 Thin Films: New Molybdenum Precursor for Low-Temperature Film Growth
Miika Mattinen, Timo Hatanpää, Tiina Sarnet,§ Kenichiro Mizohata, Kristoffer Meinander, Peter J. King, Leonid Khriachtchev, Jyrki Räisänen, Mikko Ritala,* Markku Leskelä
M. Mattinen, T. Hatanpää, Dr. T. Sarnet, Dr. P. King, Dr. L. Khriachtchev, Prof. M. Ritala, Prof. M. Leskelä
Department of Chemistry, University of Helsinki, P.O. Box 55, FI-00014, Finland E-mail: firstname.lastname@example.org
Dr. K. Mizohata, Dr. K. Meinander, Prof. J. Räisänen
Department of Physics, University of Helsinki, P.O. Box 43, FI-00014, Finland § Present address: Picosun Oy, Masalantie 365, FI-02430, Masala, Finland
Keywords: 2D materials, atomic layer deposition, MoS2, thin films
Molybdenum disulfide (MoS2) is a semiconducting 2D material, which has evoked wide
interest due to its unique properties. However, the lack of controlled and scalable methods for production of MoS2 films at low temperatures remains a major hindrance on its way to
applications. In this work, atomic layer deposition (ALD) is used to deposit crystalline MoS2
thin films at a relatively low temperature of 300 C. A new molybdenum precursor, Mo(thd)3
(thd=2,2,6,6-tetramethylheptane-3,5-dionato), is synthesized, characterized, and used for film deposition with H2S as the sulfur precursor. Self-limiting growth with a low growth rate of
approximately 0.025 Å cycle, straightforward thickness control, and large-area uniformity are demonstrated. Film crystallinity is found to be relatively good considering the low deposition temperature, but the films have significant surface roughness. Additionally, chemical composition as well as optical and wetting properties are evaluated. MoS2 films are
morphology, and crystallinity. The growth of crystalline MoS2 films at comparably low
temperatures by ALD contributes towards the use of MoS2 for applications with a limited
In the last 10 years, transition metal dichalcogenides (TMDCs) have received considerable attention as a promising material group for a variety of applications. The intriguing layered, two-dimensional (2D) crystal structures of TMDCs give birth to unique properties in thin (<10 nm) TMDC layers that are not seen in their bulk form. This is due to quantum confinement effects and the weakness of interlayer interactions in TMDCs.[1–4] To date, molybdenum disulfide (MoS2) has been the most extensively studied TMDC material.
Compared to the most well-known 2D material, graphene, which is a semi-metal, the semiconducting 2H phase of MoS2 is advantageous in having a band gap suitable for
electronic applications. In bulk form, MoS2 has an indirect band gap of 1.3 eV, which
increases as a function of decreasing film thickness. In monolayer MoS2 (thickness ~0.6 nm),
the band gap becomes direct with a width of 1.8 eV. Importantly, to meet the requirements of different applications, properties of MoS2 and other TMDCs can be tuned by controlling
the thickness, doping and alloying,[5–8] surface modification and functionalization,[9–11] strain,[12,13] and by creating heterostructures with other 2D materials.[6,14–16]
The appealing properties of TMDCs have led to a wide range of proposed applications. MoS2
has been extensively studied as a channel material in conventional field-effect transistors[17–21] as well as phototransistors and other optoelectronic devices.[16,21,22] The 2D structure of TMDCs plays a crucial role in possible applications relying on more exotic quantum phenomena, such as valleytronics.[23,24] MoS2 has also shown promise in, for example,
catalysis, batteries, photovoltaics, sensors, and medicine.
The production of high-quality, large-area MoS2 films with a thickness controllable down to a
challenge. Additionally, in many cases, the processing temperature should be kept as low as possible in order to avoid damaging sensitive substrates, such as polymers or nanostructures. Initially, flakes of monolayer MoS2 were produced from natural MoS2 crystals using
micromechanical exfoliation, a top-down method capable of producing high-quality monolayers, albeit with poor throughput as well as limited control over flake thickness and dimensions.[4,30,31] Liquid-phase exfoliation of bulk crystals, on the other hand, offers good
scalability, but often suffers from limited flake size, poor crystallinity, or contamination.[4,31,32]
Bottom-up methods offer a more controllable way to produce MoS2 films. High-quality MoS2
thin films are most commonly deposited by chemical vapor deposition (CVD) or sulfurization of metal or metal oxide thin films. The most common CVD procedure utilizes MoO3 and
sulfur as precursors.[33–36] Unfortunately, the low vapor pressure of MoO3 sets limitations to
both the deposition temperature (typically 650 to 850 C) and deposition area (typically no more than 1 cm2).[34,36] Sulfurization of Mo or MoOx films also requires high temperatures,
usually 500 to 1000 C.[36–39] Although upscaling of the sulfurization method appears to be easier compared to the MoO3-based CVD, sulfurization tends to produce films of lower
quality.[34,36,37] Other bottom-up techniques used for the deposition of thin MoS2 films include
sputtering, physical vapor transport (PVT), pulsed laser deposition (PLD), and atomic layer deposition (ALD).[43–52]
Atomic layer deposition is an inherently scalable technique that can be regarded as an advanced modification of CVD. It is based on self-limiting surface reactions of vapor-phase precursors that are alternately pulsed to substrates. In order to avoid uncontrolled gas-phase reactions, the precursor pulses are separated by purge or evacuation steps. The self-limiting reactions often allow deposition of high-quality films at comparatively low deposition temperatures, typically 100 to 400 C. ALD offers large-area uniformity, precise control over
film thickness as well as unmatched conformality, i.e. uniform thickness over substrates with complex three-dimensional shapes.[53–55] So far, ALD of MoS2 has been reported using MoCl5
with H2S,[43–46] as well as Mo(CO)6 with H2S,[47,52] H2S plasma, or dimethyl disulfide.[49–51]
The films deposited with Mo(CO)6 have mostly been amorphous due to the low deposition
temperatures of 100 to 200 C,[47,49–51] although the films deposited with H
2S plasma were
polycrystalline. Using MoCl5 and H2S, crystalline MoS2 films have been deposited by
ALD,[43–46] but a post-deposition annealing[43,46] or high deposition temperatures in excess of
500 C have still been required, in most cases, to obtain films of sufficient quality. Thus, there is a clear need to develop new ALD processes for MoS2.
In this study, we report the preparation of crystalline MoS2 films by ALD at a relatively low
temperature of 300 C, using a new molybdenum precursor, tris(2,2,6,6-tetramethylheptane-3,5-dionato)molybdenum(III), Mo(thd)3, with H2S as the sulfur precursor. We describe the
synthesis of Mo(thd)3 and other Mo(III) β-diketonates and evaluate their thermal properties.
Growth of MoS2 films shows typical characteristics of ALD: self-limited growth with linear
thickness control and excellent film uniformity. Detailed characterization provides information on film growth, morphology, crystallinity, and composition as well as optical properties and wettability. Film growth is demonstrated and studied on a range of different substrates.
2. Results and discussion
2.1. Precursor selection, synthesis, and evaluation
2.1.1. Evaluation of published MoS2 processes
We started the study by evaluating the known MoCl5+H2S process[43–46] in our commercial
hot-wall, flow-type ALD reactor. Despite testing a range of deposition conditions, for example temperatures from 150 to 500 C, we either obtained no films at all or the films were highly non-uniform in thickness across the substrates. Increasing the MoCl5 dose decreased
the film thickness close to the precursor inlet, which hints towards etching of the deposited film by MoCl5. Later, we also found that Mo(CO)6, the other molybdenum precursor used for
ALD of MoS2,[47–52] suffered from heavy precursor decomposition in our reactor already at
110 C. This was avoided by lowering the temperature below 100 C, but no film deposition was found in this case.
We attribute these results to the design of the ALD reactor used in this work, where the precursors undergo multiple collisions with hot walls and substrates, increasing the possibility of film etching and precursor decomposition. Additionally, the precursor source design based on inert gas valving may increase the likelihood of thermal decomposition compared to many other ALD reactors, where the precursors are usually heated in separate containers.
2.1.2 Synthesis and evaluation of Mo(III) β-diketonates
Due to the failures with the published processes, we searched for alternative Mo precursors. Interestingly, although metal β-diketonates are commonly used in ALD and CVD, there are, to the best of our knowledge, no reports on using Mo precursors containing only β-diketonate ligands. In general, reports of Mo(III) coordination compounds, especially β-diketonates, are rare. Compared to the more commonly investigated Mo(VI) precursors, the oxidation state +III may be beneficial, as it is closer to the oxidation state +IV in MoS2.
Mo(thd)3 was synthesized using a reaction between MoCl3(THF)3 and three equivalents of
Kthd or Lithd. Surprisingly, this simple metathesis reaction has not been previously reported for making Mo β-diketonates. After isolation and purification by sublimation, Mo(thd)3 was
obtained as dark brown, air sensitive solid with yields up to 83%. Crystal structure of the compound solved by single crystal X-ray diffraction (XRD) shows individual Mo(thd)3
molecules (Figure 1a). Detailed information on the crystal structure and its comparison to the previously reported Mo(III) β-diketonates are provided in Supporting Information.
Thermogravimetric analysis (TG) was used to evaluate thermal properties of Mo(thd)3 as well
as similarly synthesized Mo(acac)3 and Mo(hfac)3 (Figure 1b). The low residual masses of 0.3
and 2.6%, respectively, for Mo(thd)3 and Mo(hfac)3 imply evaporation of the compounds. In
agreement with previous studies, Mo(acac)3 seemed to mainly decompose, which maybe
explained by the intermolecular O···H interactions found in its crystal structure.
Three steps were found in the TG curve of Mo(thd)3: first, there was a small mass loss
between 80150 °C due to evaporation of some free Hthd. Major, 95% weight loss step associated with evaporation of Mo(thd)3, was seen at 150265 °C. At 265300 °C a small,
3% weight loss step was seen, likely due to evaporation of an oxidized species MoO2(thd)2.
The first and third steps were attributed to decomposition and oxidation of Mo(thd)3,
respectively, during loading of the TG sample in air.
The TG curve measured for Mo(hfac)3 was similar to that measured for Mo(thd)3, but the
weight losses occurred at approximately 100 °C lower temperatures. This indicates that Mo(hfac)3 is well volatile, but in our studies the thermal stability of the compound seemed to
be lower than that of Mo(thd)3. Also, for thin film growth, fluorinated ligands raise the
question of possible F contamination in the resulting films. Thus, Mo(thd)3 was chosen for the
Figure 1. Mo β-diketonates. a) Molecular structure of Mo(thd)3 solved by single crystal XRD. Thermal
ellipsoids are drawn on the 30% probability level. Hydrogen atoms are omitted for clarity. b) TG curves for synthesized Mo β-diketonates.
2.2. Film growth on silicon
Based on initial growth trials, 300 C was chosen as the most promising deposition temperature for ALD of MoS2 using Mo(thd)3 and H2S. In growth experiments on native
oxide terminated silicon, saturation of the growth rate was achieved with Mo(thd)3 and H2S
pulses of at least 0.5 and 2.0 s, respectively (Figure 2a,b). The growth rates were calculated from film thicknesses measured by energy-dispersive X-ray spectrometry (EDX), assuming smooth and uniform films with bulk density (5.06 g cm3). The saturation indicates that the
precursors react with the surface in self-limiting manner, which is characteristic for ALD. Varying the purge time after each precursor pulse between 0.5 and 2.0 s caused no change in the growth rate, which further confirms the ALD-like behavior of the process. Purge times of 1.0 s and pulse times of 0.5 s for Mo(thd)3 and 2.0 s for H2S were used in the following
depositions, unless otherwise noted.
Film thickness increased linearly with increasing number of deposition cycles, although some nucleation delay appeared to be present, as the line fitted to the thickness values did not pass through the origin (Figure 2c). Growth rate of 0.028 Å cycle and nucleation delay of 150 cycles were determined from the slope and the intersection of the fitted line with the abscissa, respectively.
The lowest temperature where film growth was observed was 250 C, where the growth rate was only approximately 0.005 Å cycle (Figure 2d). When increasing the deposition temperature, the growth rate increased up to 300 C, where the majority of depositions were performed, and then decreased again when going to 325 C. At 350 C slight Mo(thd)3
decomposition was visible in the glass source tubes of the ALD reactor, and the extent of decomposition was clearly larger at 400 C.
Figure 2. MoS2 film growth. Growth rate versus a) Mo(thd)3 and b) H2S pulse length. c) Film thickness versus
number of ALD cycles. d) Growth rate versus deposition temperature. The filled and open symbols refer to single measurements and average values, respectively. Unless otherwise noted, 2000 cycles were applied at 300 C on silicon substrates, using 0.5 s (c,d) or 1 s (b) Mo(thd)3 pulses, 2 s H2S pulses and 1 s purges.
The observed growth rate was low, approximately 0.025 Å cycle. In general, two main reasons have been proposed to limit the growth rate in ALD: steric hindrance between the adsorbed precursor molecules, and limited number of reactive sites on the surface.
Relatively low growth rates have often been observed when using bulky metal thd precursors. For example, saturated growth rates of about 0.20 Å cycle and 0.15 Å cycle were reported using Ni(thd)2 and La(thd)3, respectively, with H2S.
The much smaller growth rate found in this work suggests that the density of reactive sites is more likely the limiting factor. For many ALD oxide processes, hydroxyl (-OH) groups are the major reactive sites, whereas the analogous thiol (-SH) groups can play an important
groups, and, consequently, in the ALD growth rate of GaSx deposited from Ga2(NMe2)6 and
H2S, when increasing the deposition temperature from 125 to 225 C.
The density of thiol groups, at least on the most common, sulfur-terminated, (002) basal planes of MoS2 can be expected to be small based on the studies on MoS2 catalysts. The
edges of basal plane-terminated, typically platelike crystallites, on the other hand, contain dangling bonds and may act as reactive sites, as may also other kinds of defect sites. Thus, it is possible that the film growth proceeds mainly on the edges and defects, which could explain the slow growth.
2.3. Characterization of films deposited on silicon
The evolution of film morphology with increasing film thickness was analyzed with scanning electron microscopy (SEM, Figure 3a) and atomic force microscopy (AFM, Figure 3b). The surface remained smooth and featureless up to 250 cycles, which may be due to the nucleation delay noted above. After 500 cycles, small crystallites or particles appeared, and the film seemed to be discontinuous at this point. This is expected, as nucleation delay is often connected to island growth in ALD. The flake-like morphology with the crystallites standing up from the substrate became more pronounced with increasing number of deposition cycles. The apparent lateral grain size estimated from the SEM and AFM images increased slightly with increasing number of deposition cycles, from approximately 10 to 30 nm.
The evolution of film roughness (Figure 3c) can yield useful information on the film growth. The small grain size and considerable roughness make it difficult to determine from the SEM and AFM images when a continuous or closed film is formed, and although the morphology is also a challenge for AFM roughness measurements, the small decrease in roughness between 750 and 1000 cycles may indicate the formation of a continuous film, as demonstrated by the simulations of ALD film growth by Nilsen et al.[66,67] as well as experimental observations on HfO2 and Pt ALD films, for example.
Additional information on the surface morphology can be obtained by examination of line profiles taken from the AFM images (Figure 3d). In a film grown with 500 cycles, for example, there are height differences of up to 3 nm, which is to be compared with the average film thickness of approximately 1 nm. This shows the extent of film roughness caused by the flakes standing up from the substrate plane, which is detrimental for applications requiring smooth films, for example electronics. However, some applications, such as electrochemical
hydrogen evolution,[25,70] and batteries may also benefit from large film roughness and
films exposing the crystallite edges and interlayer spaces.
In thin film growth the film morphology is first controlled by nucleation and later by grain growth processes. Nucleation of ALD films can be sensitive to the deposition chemistry and conditions, including factors such as precursors and their pulse times, substrate and its preparation, and deposition temperature. The orientation of the formed nuclei can then affect or even determine the film morphology. Furthermore, if the film growth mainly occurs on edges and defect sites of MoS2 crystallites, as suggested in Section 2.2, this could lead to the
perceived fairly random orientation of crystallites. Thus, even if the initially formed nuclei have their basal (002) planes oriented parallel to the substrate, their orientation can change with increasing film thickness.
Figure 3. Surface morphology of MoS2 films. a) SEM images of MoS2 films grown with 250 to 4000 cycles. b)
AFM images and film roughness (Rq) of Si substrate and MoS2 films grown with 100 to 4000 cycles. c) Film
roughness versus number of deposition cycles. d) Representative AFM line profiles of Si substrate and MoS2
films grown with 500, 1000, and 2000 cycles. All of the films were deposited at 300 C on Si. 2.3.2. Crystallinity
We studied the crystallinity of the films using XRD and Raman spectroscopy. In grazing incidence XRD, a peak corresponding to the (002) plane of the desired, semiconducting 2H phase of MoS2, was detected after 1000 cycles (Figure 4a). After 4000 cycles, weak peaks
corresponding to the (100) or (101) as well as the (110) planes were also detected. The improvement of the crystallinity with increasing number of deposition cycles is evident in the decreasing width of the (002) peak.
Raman spectroscopy is a powerful method for studying TMDCs, as it can provide information on crystal structure (phase), electronic structure, strain, and film thickness, among others. The films studied with Raman measurements were deposited on 90 nm SiO2/Si substrates,
where the SiO2 layer is close to the quarter-wave thickness of the 488 nm laser, and gives a
strong signal enhancement for thin films on top, including MoS
2. We note that the film
growth was very similar on both 90 nm SiO2 and native oxide covered silicon, as will be
discussed in Section 2.4. After only 500 deposition cycles, we observed intense peaks at 384 and 406 cm1, which correspond to the E12g and A1g vibrations of 2H-MoS2, respectively
(Figure 4b).[72,75] The intensity of these two peaks did not increase monotonously with increasing film thickness, in accordance with some previous studies.[75,76] However, the intensity of the Si peak at 520 cm1, which originates from the substrate below the MoS2 and
SiO2 layers, expectedly decreased with increasing MoS2 film thickness.
Interestingly, we observed no change in the peak positions or separation (22 cm1) when the film thickness increased from approximately 1 nm (500 cycles) to 5 nm (2000 cycles). This is in contrast to the typically observed blue shift of E1
2g and red-shift of A1g peak with
decreasing film thickness in few-layer MoS2. The lack of peak shifts may result from
coexistence of MoS2 crystallites with different thicknesses, due to the initial island-like film
As we observed asymmetric broadening of the MoS2 peaks, we used the peak fitting strategy
of Mignuzzi et al. to estimate disorder in the films. In addition to the E12g and A1g modes,
three disorder-induced peaks were fitted, which originate from the transverse optical (TO, ~355 cm1), longitudinal optical (LO, ~377 cm1), and out-of-plane optical (ZO, ~412 cm1) branches at the M point of the Brillouin zone (Figure 4c). The relatively large integrated intensity of these modes compared to the E12g and A1g modes indicates the presence of
disorder in the deposited films, which is expected for a relatively low deposition temperature. The full width at half-maximum (FWHM) values of the fitted E12g and A1g components were
approximately 6 and 7 cm1, respectively, whereas those for the full peaks (i.e. without deconvolution) were around 9 cm1 for all of the measured films. Mechanically exfoliated, as well as the best CVD-grown monolayer MoS2-films deposited at 650 C or above have shown
FWHMs as low as 34 cm1.[33,78] On the other hand, for the ALD MoS2 films deposited from
MoCl5 and H2S at 475 C, the E12g FWHM was as broad as 18 cm1, which decreased by
sulfur annealing to 12 cm1 (720 C) or even 4.2 cm1 (920 C). A four-monolayer MoS2
film, produced by sulfurization of a MoOx film, yielded E12g FWHM of 6.5 cm1 at 750 C,
whereas a higher sulfurization temperature of 1000 C reduced the FWHM to 4.6 cm1. In
summary, the Raman spectra indicate comparably good crystallinity, especially considering the low deposition temperature of 300 C.
Finally, multiple measurements were performed from different positions of the ~5 cm2 SiO2
substrate (Figure 4d). Identical peak intensities at all positions, including the Si substrate peak, confirm that the films have excellent thickness uniformity, as is expected for ALD.
Figure 4. Crystallinity of MoS2 films. a) X-ray diffractograms of films grown with 500 to 4000 cycles. b)
Raman spectra of films grown with 500 to 1500 cycles. c) Peak fitting of different Raman modes in Raman spectrum of a 1000 cycle film. d) Raman spectra from different positions of a 1000 cycle film on a 2.3×2.3 cm2
substrate. All of the films were deposited at 300 C. Si and 90 nm SiO2/Si substrates were used for XRD and
Raman measurements, respectively.
We also explored how the deposition temperature affects film crystallinity. As noted earlier, self-limiting growth seemed to occur between 250 and 325 C. The crystallinity of the deposited films seemed to improve with increasing deposition temperature, based on SEM images (Figure 5a) and X-ray diffractograms (Figure 5b). Although a clear increase in grain size was evident at 350 C, and especially at 400 C, these films were not deposited under pure ALD conditions. The film deposited at 400 C consisted of thin flakes standing up from the substrate with a length of approximately 100 nm, for a nominal film thickness of about 20 nm. Deposition of highly crystalline MoS2 films by ALD appears to call for more thermally
Figure 5. Effect of deposition temperature on film crystallinity. a) SEM images and b) X-ray diffractograms of
MoS2 films grown at different temperatures on silicon using 2000 cycles.
X-ray photoelectron spectroscopy (XPS) was used to study the composition and chemical bonding on the film surface, i.e. no sputtering was done. A survey scan (Figure S2a and Table S3 in Supporting Information) revealed peaks originating from Mo, S, O, C, and Sn. Additionally, time-of-flight elastic recoil detection analysis (ToF-ERDA) provided information on film composition averaged throughout the film thickness, detecting also hydrogen and a small amount of nitrogen in addition to the abovementioned elements (Table S3 in Supporting Information). It should be noted, however, that due to the small thickness of the analyzed film (~10 nm) as well as the rough morphology, the film surface, the film-substrate interface, and the native SiO2 layer likely make a notable contribution to the
High-resolution X-ray photoelectron spectra from the Mo 3d region (Figure 6a) showed a doublet corresponding to Mo 3d5/2 at 229.9 eV and Mo 3d3/2 at 233.1 eV. The observed
binding energies are amongst those reported for thin 2H-MoS2 layers and films (231.6 to
233.2 eV for Mo 3d3/2)[39,43,44,47–49,51,52,40]. In addition, about 10% of the molybdenum was
present as oxidized MoO3 (Mo6+) with binding energies of 233.4 and 236.6 eV for Mo 3d5/2
air. The sulfur/molybdenum atomic ratio of 1.7 (ToF-ERDA) is in agreement with fairly stoichiometric MoS2 with some surface oxidation. S 2s peak was also observed near the Mo
3d doublet at 227.1 eV, in good agreement with the binding energy of S2- in 2H-MoS2.[39,43,44,47]
Binding energies of S 2p3/2 (162.7 eV) and S 2p1/2 (163.9 eV) seen in Figure 6b are also
within the range of values reported for 2H-MoS2.[39,43,44,47–49,51,52,40] Additionally, weak
doublets at 161.8 and 163.3 eV as well as 163.9 and 165.1 eV were assigned to Sn-S and C-S bonding, respectively. Carbon and oxygen were present in multiple chemical environments, as revealed by their broad peaks (Figure S2b,c in Supporting Information). It appears likely that most of the carbon, as well as the hydrogen observed by ToF-ERDA, originate from surface hydrocarbon contamination, although the presence of some residual thd ligands or their fragments cannot be excluded. The oxygen is likely due to surface oxidation, atmospheric contamination, and native SiO2 layer, the last one affecting ToF-ERDA results
A small amount of tin present in the films (approximately 13% of the amount of molybdenum) was assigned to be present as tin(IV)sulfide species (Figure 6b and Figure S2d in Supporting Information). Tin is a residue from the synthesis of the Mo(thd)3 precursor,
where metallic tin was used as a reducing agent.
Figure 6. X-ray photoelectron spectra. a) Mo 3d / S 2s region. b) S 2p region. The analyzed film was deposited
18 2.3.4. Other film properties
We also studied the wettability of the deposited films, and observed the water contact angle to increase with increasing film thickness from slightly hydrophilic (80 after 100 cycles) to hydrophobic (above 100 after 4000 cycles) as a consequence of increased roughness. More detailed results can be found in Supporting Information. Optical properties of the films deposited on glass substrates will be discussed in Section 2.4.3.
2.4. Films on other substrates
2.4.1. Film growth
We evaluated a range of different substrates to see how the film growth, surface morphology, and crystallinity are affected by the substrate. As ALD is based on surface reactions, the substrate often has an effect on the film growth in the nucleation stage, which can further alter the resulting film properties. Compared to the already discussed native oxide covered silicon, the other tested substrates can be roughly divided into three groups in terms of the growth rate (Table 1): enhanced growth with more than doubled growth rate was seen on soda lime glass, whereas smaller enhancement was found on ALD-SnS and, surprisingly, HF-treated silicon (Si-H) substrates. On the other hand, ALD-Al2O3 and ALD-Ir substrates showed inhibited
growth. On majority of the tested substrates (90 or 300 nm SiO2, borosilicate glass, sapphire,
indium tin oxide (ITO) coated glass, ALD-ZnS, and ALD-SnO2), the growth rate was similar
We speculate that the enhanced growth on soda lime glass could be due to interfacial mixing, i.e. diffusion of some of the substrate cations, especially Na, into the film. This could affect precursor adsorption and, furthermore, growth rate. We note that borosilicate glass, which was found to contain Al, B, Ba, Ca, Si, Sr, Zn, and W cations, but no alkali metals, yielded growth rate similar to silicon. We also found that film growth saturated on soda lime glass, although with longer Mo(thd)3 pulses compared to Si, with the saturated growth rate being
approximately four times that on silicon (Figure S5a,b in Supporting Information). The growth was also linear with respect to the number of deposition cycles on both silicon and soda lime glass, thus excluding nucleation effects as an explanation for the different growth rates (Figure S5c in Supporting Information).
Inhibited growth on ALD-Al2O3 may be explained by surface “poisoning” by β-diketonate
ligands, which has been found to hinder nucleation of ALD NiS and SnS on ALD-Al2O3.
appear to be unreactive towards H2S. Interestingly, film growth on sapphire (α-Al2O3) was
more facile than on amorphous ALD-Al2O3, which could be due to different bonding of the
thd-ligand to these surfaces. The inhibited growth on ALD-Ir may stem from the high catalytic activity of iridium, as decomposition of Mo(thd)3 into a carbonaceous layer on
iridium could inhibit further adsorption of the precursor, and terminate the film growth.
Table 1. MoS2 film growth rate, surface roughness, and XRD (002) FWHM on different
substrates. 2000 cycles were applied at 300 C.
Substrate Growth rate
[Å cycle] Roughness [nm] XRD (002) FWHM  Si (native oxide) 0.025±0.005 2.2 3.2 Enhanced growth Soda lime glass 0.065 (0.11a)) 2.4 2.7 ALD-SnS 0.041 -b) 2.9 Si-H 0.036 4.2 3.3
Growth rate similar to Si
SiO2 0.025 2.1 2.9 Borosilicate glass 0.025 3.7 3.0 Sapphire 0.023 2.4 4.5 ITO coated glass 0.030 -b) -c) ALD-ZnS 0.023 -b) -c) ALD-SnO2 0.026 -b) -c) Inhibited growth ALD-Al2O3 <0.005d) 1.8 -c) ALD-Ir <0.005d) -b) -c) a)With 1 s Mo(thd)
3 pulse, instead of 0.5 s; b) Not measured; c) No peak; d) Film thickness
below the detection limit of approximately 1 nm
2.4.2. Film morphology and crystallinity
In addition to the growth rate, film morphology, roughness, and crystallinity were also affected by the substrate choice. Morphology was evaluated from SEM (Figure S6 in Supporting Information) and, for selected substrates, AFM images (Figure S7 in Supporting
Information). AFM images were also used for calculating film roughness. Crystallinity was estimated from the FWHM of the (002) XRD reflection of MoS2 (Figure S8 in Supporting
Information). As is well known, peak width increases with decreasing crystallite size, although it can also be affected by other factors, such as strain.
Films on Si and SiO2 were found to be similar in terms of morphology, roughness, and
crystallinity, which is expected considering that our silicon substrates were covered by a native silicon oxide layer. Regarding the substrates with enhanced growth, films on soda lime glass had crystallinity and roughness similar to Si, when comparing films with similar thicknesses. Thus, it appears that if any mixing with soda lime glass substrate occurs, it does not deteriorate film crystallinity. The film grown on hydrogen-terminated silicon (Si-H) was the roughest out of all of the substrates studied by AFM, which may at least partially explain the somewhat higher growth rate compared to Si. In terms of crystallinity, films on Si-H and ALD-SnS also appeared to be similar to Si.
Of the substrates with growth rates similar to Si, films on borosilicate glass and sapphire showed similar and weaker crystallinity, respectively, compared to Si. The film on borosilicate glass was quite rough due to larger flakes scarcely present on the surface. For the films on ALD-SnO2, ALD-ZnS, and ITO coated glass no signs of crystallinity were detected
by XRD. On the substrates with inhibited growth (ALD-Al2O3 and ALD-Ir), no signs of
crystallinity were detected, although there were small features visible on ALD-Al2O3 in AFM
and SEM images. For some of the substrates, especially ITO coated glass and ALD-SnO2, and,
to a smaller degree, ALD-SnS, ALD-ZnS, and ALD-Ir, the inherent roughness and morphology of the substrates hindered reliable examination of the MoS2 morphology.
2.4.3. Optical properties on glass substrates
We studied the optical properties of MoS2 films deposited on soda lime and borosilicate glass
on silicon, we assume that the optical properties should also be similar. The transmittances of the bare glass substrates were quite similar to each other, as were the general shapes of the transmittance curves of the MoS2-covered substrates (Figure 7a). The two broad features
marked with asterisks at 610 and 660 nm were assigned to characteristic A and B exciton peaks of 2H-MoS2, respectively.
Using a Tauc plot we obtained an indirect band gap of 1.2 eV for a 2000 cycle film on borosilicate glass (Figure 7b), in agreement with the generally accepted value of 1.3 eV for bulk MoS2. Band gaps of 1.2±0.2 eV were measured for films of different thickness (1000 to
8000 cycles, corresponding to approximately 5 to 50 nm) on soda lime glass. Band gap determination of films thinner than about 5 nm was not successful using this method and equipment. Therefore, we were unable to observe the increase in band gap with decreasing thickness that is commonly found for few-layer MoS2.
Figure 7. Optical properties of MoS2 films. a) UV-VIS transmittance spectra for bare and MoS2-covered soda
lime and borosilicate glass substrates. b) Tauc plot for a MoS2 film on borosilicate glass. The films were
In this work, we deposited crystalline MoS2 thin films by ALD using a new molybdenum
precursor, Mo(thd)3, together with H2S at 300 C. Self-limiting growth and linear film
thickness control, characteristic of ALD, were demonstrated. We characterized the films using a variety of techniques. The films were found to be rather rough, consisting of flake-like grains with size of approximately 10 to 30 nm. Raman spectroscopy revealed the film crystallinity to be relatively good, especially taking the low deposition temperature into account. Compositional studies showed some surface oxidation and contamination, but the films themselves were estimated to be close to stoichiometric MoS2. Optical and wetting
properties of the films were also analyzed, showing properties expected for MoS2. We
deposited MoS2 films on different substrates, and although the growth was successful on most
of them, there were marked differences in the film growth, morphology, and crystallinity. The current work offers an alternative for deposition of crystalline MoS2 films at modest
deposition temperatures compared to alternative deposition methods.
4. Experimental Section
Precursor synthesis and characterization: All handling and manipulations were done under rigorous exclusion of air and moisture using standard Schlenk techniques and inert gas (N2 or
Ar) glove box. Hexane and toluene were dried over 4 Å molecular sieves while Et2O and THF
were freshly distilled from sodium benzophenone ketyl. MoCl5 (99.6%, anhydrous, Strem),
KH 30 wt-% dispersion in mineral oil (Aldrich), and Hthd (98%, Strem) were used as received. Kthd was prepared by reacting KH with Hthd in THF. MoCl3(THF)3 was prepared
by reducing MoCl5 with Sn pellets using a method modified from the one introduced by
Stoffelbach et al.
Thermogravimetric analysis was performed using a Mettler Toledo Stare system equipped with a TGA850 thermobalance. The measurements were done at atmospheric pressure using N2 (50 ml min) as the purge gas. Heating rate was 10 °C min and the sample size was
10±1 mg. Melting points were taken from the single differential thermal analysis (SDTA) data measured by the thermobalance. Mass spectra were recorded with a JEOL JMS-SX102 instrument operating in electron impact mode (70 eV) using a direct insertion probe and a sublimation temperature range of 50300 °C.
Mo(thd)3: In a 600 ml Schlenk bottle MoCl3(THF)3 (12.95 g, 30.90 mmol) was suspended in
THF (200 ml). This solution was cooled to 10 °C with an ice/acetone bath and THF solution (200 ml) of Kthd (20.59 g, 92.69 mmol) was added using a Teflon cannula and argon pressure. The solution was allowed to warm to room temperature and left to stir over night. THF was evaporated using a warm water bath and vacuum. The resulting dark brown solid was transferred into a sublimator and sublimed at 160 °C / 0.5 mbar. The sublimate being the product, Mo(thd)3, it was collected in a glove box. The yield of the highly air sensitive, dark
brown solid was 16.60 g (83%). m.p. 149 °C.
MS: m/z 647 (M+) with the correct isotopic pattern. In addition, several fragment ions were seen. Ions with oxygen, like [Mo(thd)2O2]+, [Mo(thd)2O]+, [Mo(thd)2O2 – tBu]+ and
[Mo(thd)O2]+ were also seen, but these were most likely due to exposure to air during loading
the sample into the mass spectrometer.
NMR was not resolvable because the compound was paramagnetic. Details of the crystal structure determination can be found in the Supporting Information. CCDC 1526595 contains the supplementary crystallographic data for this paper. These data can be obtained free of charge from The Cambridge Crystallographic Data Centre via www.ccdc.cam.ac.uk/data_request/cif.
Film deposition: A commercial, flow-type F-120 ALD reactor (ASM Microchemistry) was used for the deposition of MoS2 thin films under a pressure of about 5 mbar. Nitrogen (N2,
AGA, 99.999%) at a flow rate of 400 sccm was used as carrier gas as well as for purging. Mo(thd)3 was sublimed from an open glass boat held at 115 C, and pulsed with inert gas
valving. Hydrogen sulfide (H2S, Messer-Griesheim, 99.99%) was fed into the reactor through
needle and solenoid valves with its flow rate adjusted to 7 sccm during continuous flow. Purges of 1 s were used between the precursor pulses, whereas Mo(thd)3 and H2S pulse
lengths of 0.5 and 2 s were used, unless otherwise noted. Temperatures from 250 to 400 C were explored, with the optimal temperature of 300 C used in most depositions.
Films were mostly deposited on 5 × 5 cm2 silicon and soda lime glass substrates. The native
oxide of silicon was not removed, unless otherwise noted. Piranha treatment and solvent cleaning of the silicon substrates was tested, but no major difference in film growth was found; thus, the normal procedure only included removal of particles by a blow of pressurized nitrogen. Some depositions were performed on HF-treated, hydrogen-terminated silicon (Si-H), SiO2 with a thickness of 90 or 300 nm, borosilicate glass, indium tin oxide (ITO) coated
ALD films, Al2O3, SnS, and ZnS were deposited immediately before the MoS2 deposition in
the same ALD reactor, i.e. without a vacuum break.
Film characterization: Film thicknesses were measured by EDX (Oxford INCA 350 connected to a Hitachi S-4800 SEM). The EDX spectra were measured at 20 keV and an optimization procedure was used to determine the beam current as well as the spectrometer gain under the same measurement conditions. GMRFilm program was used to calculate the
film thickness and composition from the measured k-ratios of the Mo Lα and S Kα X-ray lines using the phi-rho-Z (PAP) matrix correction. Smooth and uniform films and a MoS2
bulk density of 5.06 g cm3 were assumed in the calculations. Due to the difficulty in separating the Mo and S X-ray lines, the EDX measurement uncertainty was estimated to be 20%.
Film morphology was studied by SEM (Hitachi S-4800) and AFM (Veeco Multimode V). Silicon probes with nominal tip radius of less than 10 nm (Bruker) were used for the tapping-mode AFM imaging in air. AFM images were flattened or planefitted to minimize the effects of sample tilt and scanner nonlinearity. Roughness was calculated as a root-mean-square value (Rq). Bruker Nanoscope 1.5 software was used for image modification and analysis.
Composition of the surface layers was analyzed by XPS using an Argus Spectrometer (Omicron NanoTechnology GmbH) operating at a pass energy of 20 eV. Samples were illuminated with X-rays emitted from a standard Mg source (Kα line) at a photon energy of 1253.6 eV. Binding energies were calibrated using the C 1s peak (284.8 eV) of ambient hydrocarbons, and peak fitting was done using the CasaXPS software. Film composition averaged throughout the film thickness was analyzed by ToF-ERDA using a 40 MeV 127I7+
Film crystallinity was probed with XRD (PANalytical X’Pert Pro MPD) using grazing incidence geometry (incident angle of 1) and Cu Kα radiation (λ = 1.54 Å). To determine the FWHM, XRD peaks were fit with Gaussian functions. Micro-Raman spectra were recorded in
a back-scattering scheme with a confocal Raman microscope (Horiba Jobin Yvon LabRam HR 800) using excitation at 488 nm of an argon-ion laser (2.5 mW on the sample), a 100× objective, and spectral resolution of 2 cm1. The total acquisition time was 100 s. Peak fitting was conducted using Pseudo-Voigt function implemented in OriginPro 8.6.
Optical transmission measurements using a UV-VIS spectrophotometer (Hitachi U-2000) were used to construct Tauc plots and determine the band gaps of films deposited on borosilicate and soda lime glass substrates. Resistance measurements were performed using a four-point probe (CPS probe station connected to a Keithley 2400 SourceMeter). Static water contact angles were measured with a Cam 100 instrument from KSV Instruments using de-ionised water.
Supporting Information is available from the Wiley Online Library or from the author.
The research was supported by ASM Microchemistry and the Finnish Centre of Excellence in Atomic Layer Deposition funded by Academy of Finland. Mr. Mikko Heikkilä and Dr. Marianna Kemell are thanked for assistance with the XRD and EDX measurements, respectively. Dr. Elena Cianci and Dr. Silvia Vangelista from Laboratorio MDM, IMM-CNR, Italy, are acknowledged for help in trials with the Mo(CO)6 precursor.
Received: ((will be filled in by the editorial staff)) Revised: ((will be filled in by the editorial staff)) Published online: ((will be filled in by the editorial staff))
 K. F. Mak, C. Lee, J. Hone, J. Shan, T. F. Heinz, Phys. Rev. Lett. 2010, 105, 136805.  W. Zhao, R. M. Ribeiro, G. Eda, Acc. Chem. Res. 2015, 48, 91.
 M. Chhowalla, H. S. Shin, G. Eda, L.-J. Li, K. P. Loh, H. Zhang, Nat. Chem. 2013, 5, 263.
 Y. P. V. Subbaiah, K. J. Saji, A. Tiwari, Adv. Funct. Mater. 2016, 26, 2046.  A. A. Tedstone, D. J. Lewis, P. O‘Brien, Chem. Mater. 2016, 28, 1965.
 H. Wang, H. Yuan, S. S. Hong, Y. Li, Y. Cui, Chem. Soc. Rev. 2014, 44, 2664.
 J.-G. Song, G. H. Ryu, S. J. Lee, S. Sim, C. W. Lee, T. Choi, H. Jung, Y. Kim, Z. Lee, J.-M. Myoung, C. Dussarrat, C. Lansalot-Matras, J. Park, H. Choi, H. Kim, Nat. Commun. 2015, 6, 7817.
 Y. Chen, J. Xi, D. O. Dumcenco, Z. Liu, K. Suenaga, D. Wang, Z. Shuai, Y.-S. Huang, L. Xie, ACS Nano 2013, 7, 4610.
 S. Presolski, M. Pumera, Mater. Today 2015, 19, 140.
 M. Amani, R. A. Burke, X. Ji, P. Zhao, D.-H. Lien, P. Taheri, G. H. Ahn, D. Kiriya, J. W. Ager III, E. Yablonovitch, J. Kong, M. Dubey, A. Javey, ACS Nano 2016, 10, 6535.  X. Chen, A. R. McDonald, Adv. Mater. 2016, 28, 5738.
 A. Castellanos-Gomez, R. Roldán, E. Cappelluti, M. Buscema, F. Guinea, H. S. J. van der Zant, G. A. Steele, Nano Lett. 2013, 13, 5361.
 H. J. Conley, B. Wang, J. I. Ziegler, R. F. Haglund Jr., S. T. Pantelides, K. I. Bolotin, Nano Lett. 2013, 13, 3626.
 S. Bertolazzi, D. Krasnozhon, A. Kis, ACS Nano 2013, 7, 3246.
 X. Duan, C. Wang, J. C. Shaw, R. Cheng, Y. Chen, H. Li, X. Wu, Y. Tang, Q. Zhang, A. Pan, J. Jiang, R. Yu, Y. Huang, X. Duan, Nat. Nanotechnol. 2014, 9, 1024.
 W. Zhang, Q. Wang, Y. Chen, Z. Wang, A. T. S. Wee, 2D Mater. 2016, 3, 022001.  F. Schwierz, J. Pezoldt, R. Granzner, Nanoscale 2015, 7, 8261.
 B. Radisavljevic, A. Radenovic, J. Brivio, V. Giacometti, A. Kis, Nat. Nanotechnol.
2011, 6, 147.
 J. Li, M. Östling, Electronics 2015, 4, 1033.
 Y. Yoon, K. Ganapathi, S. Salahuddin, Nano Lett. 2011, 11, 3768.
 D. Jariwala, V. K. Sangwan, L. J. Lauhon, T. J. Marks, M. C. Hersam, ACS Nano 2014, 8, 1102.
 K. F. Mak, J. Shan, Nat. Photonics 2016, 10, 216.
 D. Xiao, G.-B. Liu, W. Feng, X. Xu, W. Yao, Phys. Rev. Lett. 2012, 108, 196802.  H. Zeng, J. Dai, W. Yao, D. Xiao, X. Cui, Nat. Nanotechnol. 2012, 7, 490.
 D. M. Andoshe, J.-M. Jeon, S. Y. Kim, H. W. Jang, Electron. Mater. Lett. 2015, 11, 323.
 X. Wang, Q. Weng, Y. Yang, Y. Bando, D. Golberg, Chem. Soc. Rev. 2016, 45, 4042.  X. Yu, K. Sivula, ACS Energy Lett. 2016, 1, 315.
 K. Kalantar-zadeh, J. Z. Ou, ACS Sensors 2015, 1, 5.  Y. Chen, L. Wang, J. Shi, Nano Today 2016, 11, 292.
 K. S. Novoselov, D. Jiang, F. Schedin, T. J. Booth, V. V Khotkevich, S. V Morozov, A. K. Geim, Proc. Natl. Acad. Sci. U. S. A. 2005, 102, 10451.
 F. Bonaccorso, A. Lombardo, T. Hasan, Z. Sun, L. Colombo, A. C. Ferrari, Mater. Today 2012, 15, 564.
 X. Zhang, Z. Lai, C. Tan, H. Zhang, Angew. Chem. 2016, 128, 8960; Angew. Chem. Int. Ed. 2016, 55, 8816.
 Y.-H. Lee, X.-Q. Zhang, W. Zhang, M.-T. Chang, C.-T. Lin, K.-D Chang, Y.-C. Yu, J. T.-W. Wang, C.-S. Chang, L.-J. Li, T.-W. Lin, Adv. Mater. 2012, 24, 2320.
 H. F. Liu, S. L. Wong, D. Z. Chi, Chem. Vap. Deposition 2015, 21, 241.  M. Bosi, RSC Adv. 2015, 8, 75500.
 S. L. Wong, H. Liu, D. Chi, Prog. Cryst. Growth Charact. Mater. 2016, 62, 9.  R. Gatensby, T. Hallam, K. Lee, N. McEvoy, G. S. Duesberg, Solid-State. Electron.
2016, 125, 39.
 Y. Zhan, Z. Liu, S. Najmaei, P. M. Ajayan, J. Lou, Small 2012, 8, 966.  S. Vangelista, E. Cinquanta, C. Martella, M. Alia, M. Longo, A. Lamperti, R.
Mantovan, F. B. Basset, F. Pezzoli, A. Molle, Nanotechnology 2016, 27, 175703.  J.-H. Huang, H.-H. Chen, P.-S. Liu, L.-S. Lu, C.-T. Wu, C.-T. Chou, Y.-J. Lee, L.-J. Li,
W.-H. Chang, T.-H. Hou, Mater. Res. Express 2016, 3, 065007.
 S. Wu, C. Huang, G. Aivazian, J. S. Ross, D. H. Cobden, X. Xu, ACS Nano 2013, 7, 2768.
 M. I. Serna, S. H. Yoo, S. Moreno, Y. Xi, J. P. Oviedo, H. Choi, H. N. Alshareef, M. J. Kim, M. Minary-Jolandan, M. A. Quevedo-Lopez, ACS Nano 2016, 10, 6054.
 L. K. Tan, B. Liu, J. H. Teng, S. Guo, H. Y. Low, K. P. Loh, Nanoscale 2014, 6, 10584.  R. Browning, P. Padigi, R. Solanki, D. J. Tweet, P. Schuele, D. Evans, Mater. Res.
Express 2015, 2, 035006.
 Y. Kim, J.-G. Song, Y. J. Park, G. H. Ryu, S. J. Lee, J. S. Kim, P. J. Jeon, C. W. Lee, W. J. Woo, T. Choi, H. Jung, H.-B.-R. Lee, J.-M. Myoung, S. Im, Z. Lee, J.-H. Ahn, J. Park, H. Kim, Sci. Rep. 2016, 6, 18754.
 A. Valdivia, D. J. Tweet, J. F. Conley Jr, J. Vac. Sci. Technol. A 2016, 34, 021515.  D. K. Nandi, U. K. Sen, D. Choudhury, S. Mitra, S. K. Sarkar, Electrochim. Acta 2014,
31 146, 706.
 Y. Jang, S. Yeo, H.-B.-R. Lee, H. Kim, S.-H. Kim, Appl. Surf. Sci. 2016, 365, 160.  Z. Jin, S. Shin, D. H. Kwon, S.-J. Han, Y.-S. Min, Nanoscale 2014, 6, 14453.  S. Shin, Z. Jin, D. H. Kwon, R. Bose, Y.-S. Min, Langmuir 2015, 31, 1196.  D. H. Kwon, Z. Jin, S. Shin, W.-S. Lee, Y.-S. Min, Nanoscale 2016, 8, 7180.  J. J. Pyeon, S. H. Kim, D. S. Jeong, S.-H. Baek, C.-Y. Kang, J.-S. Kim, S. K. Kim,
Nanoscale 2016, 8, 10792.
 M. Ritala, J. Niinistö, in Chemical Vapour Deposition: Precursors, Processes and Applications (Eds.: A.C. Jones, M.L. Hitchman), Royal Society Of Chemistry, Cambridge, U.K., 2009, Ch. 4, pp. 158206.
 R. W. Johnson, A. Hultqvist, S. F. Bent, Mater. Today 2014, 17, 236.  S. M. George, Chem. Rev. 2010, 110, 111.
 T. Suntola, Thin Solid Films 1992, 216, 84.
 F. Stoffelbach, D. Saurenz, R. Poli, Eur. J. Inorg. Chem. 2001, 2699.
 A. Y. Ledneva, S. B. Artemkina, D. A. Piryazev, V. E. Fedorov, J. Struct. Chem. 2015, 56, 1021.
 CRC Handbook of Chemistry and Physics, 97th ed. (Online), CRC Press, Boca Raton, FL, http://hbcpnetbase.com, accessed: December, 2016
 N. Mahuli, S. K. Sarkar, J. Vac. Sci. Technol. A 2016, 34, 01A142.
 K. Kukli, H. Heikkinen, E. Nykänen, L. Niinistö, J. Alloys Compd. 1998, 275277, 10.  K. Knapas, M. Ritala, Crit. Rev. Solid State Mater. Sci. 2013, 38, 167.
 X. Meng, J. A. Libera, T. T. Fister, H. Zhou, J. K. Hedlund, P. Fenter, J. W. Elam, Chem. Mater. 2014, 26, 1029.
 J. V. Lauritsen, F. Besenbacher, J. Catal. 2015, 328, 49.  R. L. Puurunen, J. Appl. Phys. 2005, 97, 121301.
 O. Nilsen, O. B. Karlsen, A. Kjekshus, H. Fjellvåg, Thin Solid Films 2007, 515, 4538.  K. Kolanek, M. Tallarida, M. Michling, D. Schmeisser, J. Vac. Sci. Technol. A 2012,
 X. Jiang, T. M. Gür, F. B. Prinz, S. F. Bent, Chem. Mater. 2010, 22, 3024.  Q. Ji, Y. Zhang, J. Shi, J. Sun, Y. Zhang, Z. Liu, Adv. Mater. 2016, 6207.  PDF 00-037-1492, JCPDS-ICDD, International Center for Diffraction Data  X. Zhang, Q.-H. Tan, J.-B. Wu, W. Shi, P.-H. Tan, Nanoscale 2016, 8, 6435.
 L. Y. Khriachtchev, R. Lappalainen, M. Räsänen, Diam. Relat. Mater. 1998, 7, 1451.  H. Zhang, Y. Wan, Y. Ma, W. Wang, Y. Wang, L. Dai, Appl. Phys. Lett. 2015, 107,
 H. Li, Q. Zhang, C. C. R. Yap, B. K. Tay, T. H. T. Edwin, A. Olivier, D. Baillargeat, Adv. Funct. Mater. 2012, 22, 1385.
 X.-L. Li, X.-F. Qiao, W.-P. Han, X. Zhang, Q.-H. Tan, T. Chen, P.-H. Tan, Nanotechnology 2016, 27, 145704.
 S. Mignuzzi, A. J. Pollard, N. Bonini, B. Brennan, I. S. Gilmore, M. A. Pimenta, D. Richards, D. Roy, Phys. Rev. B: Condens. Matter Mater. Phys. 2015, 91, 195411.  Y. Yu, C. Li, Y. Liu, L. Su, Y. Zhang, L. Cao, Sci. Rep. 2013, 3, 1866.
 N. M. D. Brown, N. Cui, A. McKinley, Appl. Surf. Sci. 1998, 134, 11.
 T. J. Whittles, L. A. Burton, J. M. Skelton, A. Walsh, T. D. Veal, V. R. Dhanak, Chem. Mater. 2016, 28, 3718.
 J. Y. Kim, S. M. George, J. Phys. Chem. C 2010, 114, 17597.
 A. R. Beal, J. C. Knights, W. Y. Liang, J. Phys. C: Solid State Phys. 1972, 5, 3540.  R. A. Waldo, in Microbeam Analysis (Ed.: D.E. Newbury), San Francisco Press, San
Francisco, 1988, pp. 310–314.
 J. Jokinen, J. Keinonen, P. Tikkanen, A. Kuronen, T. Ahlgren, K. Nordlund, Nucl. Instruments Methods Phys. Res. Sect. B 1996, 119, 533.